Statistical inferences in material selection of a polymer
matrix for natural fiber composites
M. Noryani1), 2), 3), S.M. Sapuan1), 4), *), M.T. Mastura3), 5), M.Y.M. Zuhri1), E.S. Zainudin1)
Abstract: In this paper, statistical inferences in material selection of polymer matrix for natural fiber
composite are presented. Hypothesis testing and confidence interval were used to evaluate the suita bility of the sample for use as a matrix in natural fiber reinforced composites. The screening process for material selection was carried out using a stepwise regression method. Then, the ranking process in ma terial selection was conducted using an estimation of performance score (PS) for mechanical pro perties such as impact strength (IS), elongation at break (E) and tensile strength (TS). Ten types of polymer were involved in the study. The final selection revealed that polyamide (PA6), polyurethanes (PUR) and polypropylene (PP) are the potential candidates to manufacture handbrake levers according to IS, E and
TS, respectively. Here, it was found that the score for Tp (thermoplastic) is better than Ts (thermoset) in
terms of IS. In contrast, the Ts offered a better score result than, Tp, with respect to E and TS. The results of statistical measurements using statistical modelling prove that the data analysis can be used as a part of the decision making in material selection.
Keywords: material selection, polymer matrix, stepwise regression, hypothesis testing, confidence interval.
Wnioskowanie statystyczne w wyborze materiału osnowy polimerowej
kompozytów z włóknami naturalnymi
Streszczenie: Opisano wnioskowanie statystyczne dotyczące wyboru materiału osnowy polimerowej
kompozytu z włóknami naturalnymi. Testy hipotez statystycznych i przyjęte przedziały ufności służy ły do oceny próbki pod względem przydatności do zastosowania w charakterze osnowy polimerowej w kompozycie wzmocnionym włóknem naturalnym. Selekcji materiałów dokonano przy użyciu meto dy regresji krokowej, następnie uszeregowano wybrane materiały z wykorzystaniem rankingu oceny (PS) właściwości mechanicznych, takich jak: udarność (IS), wydłużenie przy zerwaniu (E) i wytrzy małość na rozciąganie (TS). Wyselekcjonowano wstępnie 10 rodzajów polimerów zaliczanych do grup polimerów termoplastycznych (Tp) i termoutwardzalnych (Ts). Wnioskowanie statystyczne wykazało, że poliamid (PA6), poliuretany (PUR) i polipropylen (PP) są potencjalnie korzystnymi osnowami poli merowymi do wytwarzania dźwigni hamulca ręcznego. Stwierdzono, że polimery z grupy Tp wyka zują lepszą udarność niż polimery z grupy Ts. Natomiast materiały Ts charakteryzują korzystniejsze wartości wydłużenia przy zerwaniu i wytrzymałości na rozciąganie niż ich odpowiedniki z grupy Tp. Wyniki przeprowadzonej analizy danych z zastosowaniem modelowania statystycznego dowodzą, że metoda ta może być pomocna przy wyborze materiału odpowiedniego do planowanej aplikacji.
Słowa kluczowe: wybór materiału, osnowa polimerowa, regresja krokowa, testowanie hipotez, prze
1) Universiti Putra Malaysia, Department of Mechanical and Manufacturing Engineering, Advanced Engineering Materials and
Composites Research Centre, 43400 UPM Serdang, Selangor, Malaysia.
2) Universiti Teknikal Malaysia Melaka, Faculty of Mechanical Engineering, Hang Tuah Jaya, 76100 Durian Tunggal, Melaka,
3) Universiti Teknikal Malaysia Melaka, Centre of Advanced Research on Energy, Hang Tuah Jaya, 76100 Durian Tunggal, Mela
4) Universiti Putra Malaysia, Institute of Tropical Forestry and Forest Products (INTROP), Laboratory of Biocomposite Technolo
gy, 43400 UPM Serdang, Selangor, Malaysia.
5) Universiti Teknikal Malaysia Melaka, Faculty of Mechanical and Manufacturing Engineering Technology, Hang Tuah Jaya,
76100 Durian Tunggal, Melaka, Malaysia.
Recent studies discuss the ability of polymer compo site to replace metalbased material, especially in the auto motive and construction industries. Many research ers have put forward the capabilities, suitability and af fordability of natural fibers as reinforcement agents for the polymer matrices. Natural fiber reinforced polymer composites had a good performance score with regard to their physical, mechanical and environmental pro perties when used in manufacturing automotive compo nents such as clutch pedal, car front hood, buggy bonnet, bumper beam, car roof, brake lever and antiroll bar [1–7]. As the materials are from natural sources, they can of fer an economical outflow, lightweight, environmentally friendly materials and a biodegradable effect [5, 8–13]. However, the poor dimensional stability and high mois ture absorption become a problem to these materials . There are many treatments that can increase the strength connection between the natural fiber and polymer ma trix [15–19] to produce a valuable polymer composite, es pecially in the automotive industry. Generally, thermo plastic (Tp) and thermoset (Ts) materials are the polymers used in many applications. Recently, there is a research trend in the automotive industry to produce lightweight vehicles to save energy consumption [20, 21]. Many stud ies have reported a good connection between natural fiber and polymer matrix based on the chemical composition as a better composite in automotive applications [22–24]. In addition, the combination also provides a balanced score for mechanical, thermal and electrical pro perties [25–27].
In general, the engineering plastics industry confirms the advantages of the product, such as it is lightweight, transparent, economical to produce, selflubricates, has low water absorption and good resistance to corrosion, and design flexibility [28–30]. However, Tp and Ts have their own pros and cons. Fast processing, highly recy clable, high impact resistance, chemical resistance and ecofriendly manufacturing are the advantages of Tp. However, generally, Tp is more expansive and melts if heated. In contrast, Ts is more resistant to high tempera ture, has a highly flexible design, excellent aesthetic ap pearance, high level of dimensional stability and is cost effective. The disadvantages of Ts are that it is unrecycla ble, difficult to surface finish, cannot be remolded or re shaped, and has a lower production rate due to its lengthy cure time [31–33]. In reality, there are variable and incon sistent conclusions about Tp and Ts in different applica tions. It is known that Tp is tougher than Ts because of the structure of the polymer itself. Chung  also claimed that the manufacturing time of Tp is shorter than that of Ts. Another study found that the mechanical properties, such as tensile strength, of Ts are better than those of Tp . Although a number of investigations have reported interesting results for Tp and Ts, no study has examined their performance by using statistical inferences such as hypothesis testing and confidence interval.
In material selection, numerous multicriteria decision making (MCDM) tools can be used, such as Analytical
Hierarchy Process, Analytical Network Process, Multi attribute Utility Theory, Preference Selection Index, Technique of Ranking Preferences by Similarity of the Ideal Solution and Quality Function Deployment. In practice, these tools have their own strengths and limita tions on screening and ranking methods in the process to select the best material [36, 37]. The major problem in the conventional MCDM method is inconsistent judgement and preference subjectivity over the process selection. For example, there is no standard measurement for the weighting process in Analytical Hierarchy Process and Analytical Network Process [36, 38]. Some of the tools are only able to deal with qualitative data, which is also an issue in material selection . The final decision is af fected by the limitations of these tools. However, a recent study by Noryani et al.  introduced a novel statistical framework by using stepwise regression on the screen ing process. This approach is proven to finalize the best natural fiber in automotive application . Statistical an alyzes such as estimation, error analysis, hypothesis test ing and confidence interval are the alternative measure
Materials ranking methods Optimization methods Multiple criteria decision-making methods Multiple objective decision making Fuzzy multiple attribute decision making Multiple attribute decision making Statistical analysis Genetic algorithm Computer simulation Mathematical programming Materials screening methods
Cost per unit property method Chart (Ashby’s method) Artificial intelligence method Materials in product selection tool Questionnaire method Stepwise regression Neural network Knowledge-based system Case based reasoning Computer aided material selection system
Fig. 1. Classification of: a) screening, b) ranking methods in ma-terial selection 
ments in the optimization method to rank the material’s performance. In this study, the performance score (PS) is measured by using equation (1), where
xiis the mechani cal properties of the polymer matrix. This innovative con tribution by using statistical inferences in material selec tion is shown in Fig. 1. To demonstrate the potential of this novel approach to screening and ranking methods as well as its suitability for material selection of the polymer matrix of an automotive component, the stepwise regres sion of polymer matrix data is studied and the significant statistical model for each polymer matrix is presented. Hypothesis testing and confidence interval are discussed as inferential analysis from the sample to estimate the PS using a constructed statistical model to make the final de cision. This approach can give extra information and in crease the decision maker’s confidence to select the most potential candidate to manufacture a handbrake lever for car parking, as in the case study.
i = 1,2,…,n (1)
The improvement using statistical inferential analysis in a statistical framework on previous studies is shown in Fig. 2.
Material selection of Tp and Ts
The material selection process is an important stage in engineering applications, especially in product devel opment for longterm success . The engineer should select the most suitable material that performs well and can easily be commercialized. To avoid major loss dur ing product design testing, the material selection pro cess is the critical part of the manufacturing process . Moreover, in this study, secondary data about the poly mer matrix of thermoplastic and thermoset plastic from previous works is utilised, as shown in Table 1.
All the polymer in this study are hydrophobic poly mers because this polymer used natural fiber as the rein forcement agent to the composite. The composite should water resistant in automotive application to increase the strength of the properties. In this case, there are several processes used to prepare this type of polymer, injection molding, extrusion, pultrusion and hand layup are the common methods used in research area. This data set is used to select the most suitable polymer to manufacture a handbrake lever, as shown in Fig. 3, for automotive in dustry application as the case study.
Mean (µ) and standard deviation (σ) are the nor mal statistical measurements used in previous studies [49–51]. Here, minimum, middle and maximum values
are used for mechanical properties of the Tp and Ts. The framework introduced previously by Noryani et al.  is used for the screening process, which involves an other statistical measurement such as correlation (r), de termination of coefficient (R2), adjusted determination
coefficient (AdjR2) or variance inflation factor (VIF) to
identify the best model of the polymer. Then, a com parison between the alternative polymers via an esti mation process using statistical modelling is performed. Okayasu et al.  mentioned, estimation using statisti cal analysis can give a better result compare to the com pound law. Ttest statistics are used in hypothesis test ing and confidence interval to confirm the successful inferential analysis to draw a conclusion about the per formance of the Tp and Ts.
Inferential analysis Estimation Hypothesis testing Confident interval
Fig. 2. Additional information for final decision on material se-lection
T a b l e 1. The properties of thermoplastic and thermosetting [4, 17, 30, 43–46]
Polymer Density (D) g/cm3 modulus, (YM) Young’s GPa Tensile strength, (TS) MPa Elongation at break, (E) % Impact strength, (IS) J/m2 Water absorp tion, (WA) 24 hours PP 0.86 0.89 0.90 0.91 0.92 0.95 1.36 1.40 1.60 1.80 26.0 33.7 34.5 36.0 41.4 15.0 43.0 58.1 73.2 100.0 24.40 85.05 145.70 206.35 267.00 0.010 0.010 0.015 0.02 0.02 PS 1.04 1.04 1.05 1.06 1.06 3.14 3.57 4.00 4.50 5.00 25.0 38.1 51.1 60.1 69.0 12.0 16.5 21.0 23.0 25.0 1.0 1.1 1.0 1.1 1.0 0.03 0.04 0.06 0.08 0.10 HDPE 0.94 0.95 0.96 0.96 0.97 0.40 0.76 0.95 1.00 1.50 14.5 22.0 26.3 32.0 38.0 200 745 1000 1120 1290 26.7 288 548 808 1068 0.01 0.01 0.02 0.02 0.01 LDPE 0.91 0.92 0.93 0.93 0.94 0.06 0.14 0.22 0.31 0.38 7 17 40 43 78 100 375 650 675 700 854 900 930 950 1000 0.015 0.010 0.015 0.010 0.015 TPU 1.12 1.15 1.18 1.21 1.24 1.31 1.50 1.69 1.88 2.07 31.0 38.8 46.5 54.3 62.0 60 182.5 305 427.5 550 9.42 16.80 24.21 31.60 39.00 0.15 0.16 0.17 0.18 0.19 PA6 1.120 1.125 1.130 1.135 1.140 2.80 2.85 2.90 2.95 2.90 35 39 43 61 79 38.8 59 80 100 120 42.7 72 101 130.5 160 1.30 1.43 1.55 1.68 1.80 PR 1.2 1.3 1.4 1.4 1.5 2.0 2.5 3.3 3.9 4.5 40 52.5 65 77.5 90 2 2.2 2.4 2.5 2.6 15 91 167 243 320 0.10 0.15 0.20 0.25 0.30 VE 1.20 1.25 1.30 1.35 1.40 3.10 3.27 3.45 3.62 3.80 69 72.5 76 79.5 83 4.0 4.7 5.5 6.2 7.0 250 0.10 0.05 0.10 0.15 0.20 ER 1.10 1.20 1.25 1.30 1.40 3.0 3.7 4.5 5.2 6.0 35 51 67 83 100 1.0 2.5 3.5 4.7 6.0 n/a 0.10 0.20 0.25 0.30 0.40 PUR 1.04 1.06 1.09 1.10 1.13 4.09 4.15 4.20 4.25 4.30 14 39 52 69 75.8 3.0 4.5 6.0 8.0 10.0 n/a 0.10 0.10 0.15 0.20 0.20 PP: polypropylene, PS: polystyrene, HDPE: highdensity polyethylene, LDPE: lowdensity polyethylene, TPU: thermoplastic polyuretha ne, PA6: polyamide, PR: polyester resin, VE: vinyl ester resin, ER: epoxy resin, PUR: polyurethanes.
Hypothesis testing and confidence interval
Hypothesis testing is one of the inferential statistics that can be used to make a conclusion about the popula tion based on a sample. In this study, hypothesis testing
is used to verify the performance of Tp and Ts. There are five command steps in hypothesis testing, which are: write the null and alternative hypothesis, perform the statistics testing, find the critical point and decide the re gion, finalise the decision making and, lastly, make a con
clusion. All the calculations and conclusions in this study are based on α = 0.05 (5% standard error) significant value and 95% confidence interval. The onetailed test is used where the hypothesis condition shows that Tp is better than Ts. Otherwise, the conclusion is that Ts perform bet ter than Tp. Equations (2) to (4) are used to perform the hypothesis testing and confidence interval.
(4) where: – sample mean of Tp properties, – sample mean of Ts properties, µTp – population mean of Tp prop erties, µTs – population mean of Ts properties, STp – stan dard deviation of Tp, STs – standard deviation of Ts, Sp – pooled standard deviation for two samples, nTp – number of samples for Tp, nTs – number of samples for Ts.
RESULTS AND DISCUSSION Best model of polymer matrix using stepwise regression
Table 2 shows the best statistical model with significant mechanical properties with an excellent AdjR2 that de
scribed the variation of PS. This variation is explained by the significant mechanical properties. For example, the third model proposed by stepwise regression for PP men tioned that 99.9% of the variation of PS is explained by IS,
E and TS. This new approach was proposed in a previous
study by Noryani et al.  to select the natural fiber com posite. Another previous study reported significant ten sile and flexural properties of a kenaf reinforced polypro pylene composite using stepwise regression . In this paper, the only significant mechanical property for ther mosetting PR was WA, while the other mechanical prop erties did not contribute to the model for estimation pur poses. Each polymer has its own significant mechanical properties. For estimation purposes, the most significant mechanical properties equation of the polymer where IS,
E and TS are chosen to be compared in the selection pro
cess. For example, IS is the significant mechanical prop erty for PP, HDPE, LDPE and PA6. Therefore, this model is used to estimate the PS by substituting the product de sign specification of IS in manufacturing the handbrake lever. The process is also applied for E and TS for the alternative polymer. The quality of the material’s inter face strength is evaluated by using an estimation process through the statistical model .
Material selection based on performance of mechanical properties
IS, E and TS are the most significant mechanical proper
ties in the polymer model. Here, the product design speci fication for manufacturing a handbrake lever of IS, E and
TS is referred [43, 48, 54]. Selection of the materials should
be consistent with the industry declaration on product de sign specification . One of the materials used to manu facture the handbrake lever is structural steel S235 . The properties of S235 for IS, E and TS are 27 J/m2, 25%
and 460 MPa, respectively. Figures 4, 5 and 6 show the PS score according to IS, E and TS. From the result, the PA6 is the best material to manufacture the handbrake lever, if the focus of the automotive industry for the component is on IS. Surprisingly, PP, HDPE and LDPE only score around 26 to 27 of PS compared to PA6, which scored 61.61. Based on Fig. 5, there are six polymers involved in estimation on
PS according to elongation at break of that material. This
score can show the capability of a material to maintain its shape without crack formation. Both thermoset plas tics, which are PUR (31.12) and ER (29.28), score the highest for PS compared to the other thermoplastic. In Fig. 6, the thermoplastic materials such as PP (512.48), PS (509.57) and HDPE (501.48) perform better on PS (according to TS) com
Fig. 3. Example of a hand-brake lever for: a) Suzuki Maruti, b) Proton Wira [47, 48]
T a b l e 2. The best model with significant mechanical properties using stepwise regression
Polymer Model Mechanical properties R2 AdjR2 Standard
error P-value Equation
PP 1 IS 0.999 0.998 6.625 0.000 y = 37.96 + 1.388 IS 2 IS, E 1.0 0.999 0.701 0.000 y = 23.658 + 0.905 IS + 1.465 E 3 IS, E, TS 1.0 0.999 0.034 0.000 y = 0.8798 + 1.009 IS + 0.965 E + 1.116 TS PS 1 TS 1.0 0.999 0.512 0.000 y = 9.04 + 01.342 TS 2 TS, E 1.0 0.999 0.074 0.000 y = 4.945 + 1.097 TS + 0.822 E HDPE 1 TS 0.992 0.984 120.691 0.001 y = 987.805 + 91.679 TS 2 TS, E 0.999 0.999 39.516 0.001 y = 695.109 + 51.609 TS + 0.886 E 3 TS, E, IS 1.0 0.999 0.175 0.000 y = 0.072 + 1.09 TS + E + 0.999 IS LDPE 1 E 0.994 0.988 42.023 0.001 y = 823.594 + 1.283 E 2 E, IS 1.0 0.999 7.182 0.000 y = 515.742 + 0.973 E + 1.612 IS 3 E, IS, TS 1.0 0.999 0.040 0.000 y = 0.973 + E + 1.002 IS + TS TPU 1 WA 1.0 0.999 0.007 0.000 y = 1965.146 + 13787.6 W PA6 1 IS 0.998 0.997 6.307 0.000 y = 27.683 + 2.075 IS 2 IS, TS 1.0 0.999 0.302 0.000 y = 15.114 + 1.722 IS + 0.94 TS PR 1 WA 1.0 0.999 0.086 0.000 y = 18.49 + 268.2 W VE 1 YM 1.0 0.999 0.040 0.000 y = 2.411 + 25.742 YM ER 1 TS 1.0 0.999 0.140 0.000 y = 0.767 + 1.13 TS 2 TS, E 1.0 0.999 0.042 0.000 y = 2.402 + 1.049 TS + 1.075 E PUR 1 TS 1.0 0.999 0.840 0.000 y = 5.981 + 1.115 TS 2 TS, E 1.0 0.999 0.023 0.000 y = 5.069 + 1.002 TS + 1.042 E
pared to the thermoset plastics. It is also noted that PA6 (447.51) scores the lowest PS on this mechanical property. This is similar to results found by AlOqla and Sapuan , where PP offered a better result for use in natural fi ber reinforced composite under uncertain environments. In contrast, Mansor et al.  suggested that PP is the second candidate to be used for a handbrake lever when using the analytic hierarchy process. The variation on the estimation of PS is represented by the error bar plotted in Fig. 4, Fig. 5 and Fig. 6. It indicates the uncertainty in the measured ap proximation values. In a recent study, the error bar was an
informative tool to show the goodness of fit or dispersion of the data set [55, 56]. In detail, statistical testing such as hypothesis testing, confidence interval and ttest should be performed to draw the final conclusion.
Statistical inference on mechanical properties of Tp and Ts
In this section, hypothesis testing is used as additional information to support the final decision making based on the earlier section where hypothesis testing can con
PP HDPE LDPE PA6
PS 0 10 20 30 40 50 60 70 80 0 5 10 15 20 25 30 35
PP PS HDPE LDPE ER PUR
PS 380 400 420 440 460 480 500 520 540
PP PS HDPE LDPE PA6 ER PUR
Fig. 4. The estimation of PS for the alternatives with regard to impact strength (IS)
Fig. 5. The estimation of PS for the alternatives with regard to elongation at break (E)
POLIMERY 2020, 65, nr 2 111
firm the validity of prediction by using an appropriate sample to draw a conclusion in this study. Moreover, confidence interval states the accepted range with 95% confident level on mechanical properties involved in this study. The hypothesis testing and confidence interval are performed for three selected mechanical properties, impact strength (IS), elongation at break (E) and tensile strength (TS). Table 3 shows the mean ( ), sample stan dard deviation (s) and number of samples (n) for thermo plastic and thermoset plastic.
Based on the result shown in Table 4, it can be con cluded that Tp offers better IS value than Ts, due to in sufficient evidence to reject H0. Total energy absorbed by the material before it cracks or fails indicated the mean ing of IS . As the result, Tp has a higher IS compared to Ts. In this case, Tp has better ability to absorb the en ergy during the material’s failure. This finding is con
sistent with the finding in previous section: IS obtained insignificant mechanical properties in statistical model ling for Ts candidates. There are no Ts candidates plotted in Fig. 5, although the hypothesis testing for E concluded that the E of Ts is better than that of Tp. Based on calcu lated ttest (1.811), the value fall in the critical region and over the critical point (1.697), as confirmed by tabulated
ttest with standard error (α = 0.05) and degree of freedom
(df = nTp + nTs – 2). At this stage, the evidence to reject H0 for E hypothesis testing is sufficient. Similarly, the TS for Ts is better than that for Tp. In other words, Ts is tough er and stronger than Tp. This is due to the natural be havior of this polymer, which has a strongly crosslinked molecular structure compared to the linear structure of Tp [34, 58]. Moreover, this polymer has not melted, and so the shape of items made from it would not change if heated. Similar to Okayasu et al., the tensile strength of epoxy was found to be twice as good as the other ther moplastics such as PA6 and poly(phenylene sulphide) (PPS) for carbon fiber reinforced polymer. Sivakumar
et al.  found that the tensile strength and modulus of
Tsbased material is higher than Tpbased material for a hybrid composite. In general, the mean score of TS for Ts is higher compared to that of Tp, 64.54 and 40.74, as shown in Table 4.
PP HDPE LDPE PA6
PS 0 10 20 30 40 50 60 0 5 10 15 20 25 30
PP PS HDPE LDPE ER PUR
PS 380 400 420 440 460 480 500 520 540
PP PS HDPE LDPE PA6 ER PUR
Fig. 6. The estimation of PS for the alternatives with regard to tensile strength (TS)
T a b l e 3. Statistical measurement of polymer for IS, E and TS
Polymer measurementStatistical IS E TS
Thermoplastic, Tp 291.121 305.486 40.736 sTp 378.193 367.019 17.589 n 29 29 29 Thermoset, Ts 167.2 4.415 64.54 sTs 120.483 2.299 21.167 n 20 5 20
T a b l e 4. Hypothesis testing between thermoplastic and thermoset plastic according to mechanical properties
properties Impact strength Elongation at break Tensile strength
1. Hypothesis H0 : µTp ≥ µTs H1 : µTp < µTs 2. Test statistics t = 1.413 t = 1.811 t = 4.284 3. Critical region Critical point: tα, df(nTp + nTs – 2) = t0.05, 47 = 1.68 1.684 Critical point: tα, df(nTp + nTs – 2) = t0.05, 32 = 1.697 1.697 Critical point: tα, df(nTp + nTs – 2) = t0.05, 47 = 1.684 1.684
4. Decision making Reject H0 if t-statistic fall in the region
Do not reject H0 Reject H0 Reject H0
Generally, confidence interval gives a range value of
IS, E and TS from the data collected for Tp and Ts. Here,
there is a 95% confidence interval that the value of IS,
E and TS of Tp and Ts is between (23.81, 271.65), (18.94,
583.20) and (14.45, 33.16), respectively. By using Eq. (3) and information from Table 3, detailed calculation is shown in Table 5.
Overall, 95% of the general impact strength of the poly mer is distributed between 23.811 J/m2 and 271.653 J/m2.
In this case, zero impact to 271.653 J/m2 are the range of
the impact strength of polymer are distributed. For elon gation at break, the distribution is between 18.941% and 583.200% and, lastly, with the same confidence interval, which is 95% of the tensile strength, the distribution is between 14.446 MPa and 33.162 MPa.
The evaluation of mechanical properties for 10 types of polymer in material selection by using statistical model ling was successfully achieved in this work. Additional information from statistical measurement such as esti mation, hypothesis testing and confidence interval in this study was used to demonstrate the material’s per formance effectively for each candidate throughout the polymer selection process. It can be concluded here that proper selection of polymers is dependent on mechani cal properties that influence the statistical modelling for estimation, hypothesis testing and confidence interval. This work can act as a guideline for the selection of the most suitable polymer candidate for an engineering ap plication. The results showed that:
– hypothesis testing and confidence interval results achieved a good agreement with the theory of thermoset and thermoplastic materials and this led to the final deci sion making on material selection;
– impact strength, elongation at break and tensile strength of the polymer were the three most important mechanical properties shown by the statistical modelling;
– the most suitable candidates to manufacture the handbrake lever are PA6 if based on impact strength, PUR on elongation at break and PP on tensile strength;
– thermoset plastic offers better results than ther moplastic for tensile strength and elongation at break, whereas thermoplastic exhibits better impact strength than thermoset.
The authors would like to thank Universiti Putra Malaysia for the opportunity to conduct this study as well as Universiti Teknikal Malaysia Melaka and the Ministry of Education of Malaysia for providing the scholarship award and grant scheme Hi-COE (6369107) to the principal author in this project.
 Furtado S.C.R., Araújo A.L., Silva A. et al.: International
Journal of Automotive Composites 2014, 1, 18.
http://dx.doi.org/10.1504/IJAUTOC.2014.064112  Hambali A., Sapuan S.M., Ismail N., Nukman Y.:
Journal of Central South University of Technology 2010, 17, 244.
 Ishak N.M., Malingam S.D., Mansor M.R.: International
Journal of Materials and Product Technology 2016, 53, 267.
 Mansor M.R., Hambali A., Azaman M.D. et al.:
International Symposium on the Analytic Hierarchy Process 2013, pp. 1–8.
 Mastura M.T., Sapuan S.M., Mansor M.R., Nuraini A.A.: The International Journal of Advanced
Manufacturing Technology 2017, 89, 2203.
 Mayyas A., Shen Q., Mayyas A. et al.: Materials and
Design 2011, 32, 2771.
http://dx.doi.org/10.1016/j.matdes.2011.01.001  Sapuan S.M.: Assembly Automation 2005, 25, 146.
 Aghajani Mir M., Taherei G.P., Sulaiman N.M.N. et
al.: Journal of Environmental Management 2016, 166, 109.
http://dx.doi.org/10.1016/j.jenvman.2015.09.028  AlOqla F.M., Sapuan S.M., Ishak M.R., Nuraini A.A.:
Journal of Composite Materials 2015, 50, 543.
 ALOqla F.M., Sapuan S.M.: The Journal of The
Minerals, Metals & Materials Society 2015, 67, 2450.
 Altay L., Atagur M., Akyuz O. et al.: Polymer
Composites 2017, 39, 1.
 Sahari J., Sapuan S.M., Zainudin E.S., Maleque M.A.:
Materials and Design 2013, 49, 285.
http://dx.doi.org/10.1016/j.matdes.2013.01.048 T a b l e 5. Confidence interval of mechanical properties for
properties 95% confidence interval
 Verrey J., Wakeman M.D., Michaud V., Månson J.A.E.:
Composites Part A: Applied Science and Manufacturing
2006, 37, 9.
http://dx.doi.org/10.1016/j.compositesa.2005.05.048  Jumaidin R., Sapuan S.M., Jawaid M., Ishak M.R.:
International Journal of Biological Macromolecules 2017, 97, 606.
 Bienias B., Michalski W., Wagner L.: Polimery 2019,
 Amel B.A., Paridah M.T., Sudin R. et al.: Industrial
Crops and Products 2013, 46, 117.
 Gurunathan T., Mohanty S., Nayak S.K.: Composites
Part A: Applied Science and Manufacturing 2015, 77, 1.
http://dx.doi.org/10.1016/j.compositesa.2015.06.007  Zhao Y.W., Gu Y.Z., Huang P.: Polymer Composites
2017, 39, 1.
 Ilyas R.A., Sapuan S.M., Ishak M.R., Zainudin E.S.:
Carbohydrate Polymers 2018, 202, 186.
 Calado E.A., Leite M., Silva A.: Journal of Cleaner
Production 2018, 186, 113.
 Lyu M.Y., Choi T.G.: International Journal of Precision
Engineering and Manufacturing 2015, 16, 213.
 Azammi A.M.N., Sapuan S.M., Ishak M.R., Sultan M.T.H.: Fibers and Polymers 2018, 19, 446.
 Radzi A.M., Sapuan S.M., Jawaid M., Mansor M.R.:
Fibers and Polymers 2017, 18, 1353.
 Väisänen T., Das O., Tomppo L.: Journal of Cleaner
Production 2017, 149, 582.
 Ilyas R.A., Sapuan S.M., Ishak M.R., Zainudin E.S.:
International Journal of Biological Macromolecules 2019, 123, 379.
 Punyamurthy R., Sampathkumar D.: International
Journal of Sciences: Basic and Applied Research 2014, 18,
 Rajesh M., Pitchaimani J., Rajini N.: Procedia
Engineering 2016, 144, 1055.
 Hufenbach W., Gude M., Geller S., Czulak A.: Polimery
2013, 58, 473.
 Salasinska K., Polka M., Gloc M., Ryszkowska J.:
Polimery 2016, 61, 255.
 Peters E.N.: “Thermoplastics, Thermosets, and Elastomers – Descriptions and Properties” in “Mechanical Engineers’ Handbook” 4th ed. (Ed. Kutz M.), John Wiley & Sons Inc, Selkirk, New York 2015.  Abishera R., Velmurugan R., Nagendra Gopal K.V.:
Polymer Engineering Science 2018, 58, 189.
 Singh A.K., Panda B.P., Mohanty S. et al.:
Polymer-Plastics Technology and Engineering 2018, 57, 903.
http://dx.doi.org/10.1080/03602559.2017.1354253  Tatsuno D., Yoneyama T., Kawamoto K., Okamoto
M.: Polymer Composites 2016, 39, 2571. http://dx.doi.org/10.1002/pc.24242
 Chung D.D.L.: Materials Science and Engineering: R:
Reports 2017, 113, 1.
 Okayasu M., Tsuchiya Y., Arai H.: Journal of Materials
Science Research 2018, 7, 12.
 Velasquez M., Hester P.T.: International Journal of
Operations Research 2013, 10, 56.
 Shah D.U.: Materials and Design 2014, 62, 21. http://dx.doi.org/10.1016/j.matdes.2014.05.002
 Ahmed Ali B.A., Sapuan S.M., Zainudin E.S., Othman M.: Journal of Cleaner Production 2015, 107, 557. http://dx.doi.org/10.1016/j.jclepro.2015.05.084
 Das A., Kumar A.: Journal of Mechanical and Civil
Engineering 2015, 12, 82.
 Noryani M., Sapuan S.M., Mastura M.T. et al.: Fibers
and Polymers 2018, 19, 1039.
 Noryani M., Sapuan S.M., Mastura M.T. et al.: Journal
of Materials Research and Technology 2019, 8, 2865.
 Yousefpour M., Rahimi A.: Materials and Design 2014,
http://dx.doi.org/10.1016/j.matdes.2013.08.017  “Granta Design, CES Edupack” 2013.
 Mastura M.T., Sapuan S.M., Mansor M.R., Nuraini A.A.: International Journal of Precision Engineering and
Manufacturing-Green Technology 2017, 5, 111.
 Sivakumar D., Ng L.F., Lau S.M., Lim K.T.: J.ournal of
Polymer Environment 2017, 26, 499.
 Stirna U., Beverte I., Yakushin V., Cabulis U.: Journal
of Cellular Plastics 2011, 47, 337.
 Mansor M.R., Sapuan S.M., Zainudin E.S. et al.:
Materials and Design 2013, 51, 484.
 Patel M.V., Sarawade S.S.: “Design and Weight Optimization of Parking Brake Lever” in 3rd
International Conference on Emerging Trends in Engineering and Management Research, Pune, India, July 30, 2017, p. 367.
 Fayazbakhsh K., Abedian A., Manshadi B.D., Khabbaz R.S.: Materials and Design 2009, 30, 4396. http://dx.doi.org/10.1016/j.matdes.2009.04.004
 Linul E., Marsavina L., Voiconi T., Sadowski T.:
Journal of Physics: Conference Series 2013, 451, 1.
http://dx.doi.org/10.1088/17426596/451/1/012002  Van de Velde K., Kiekens P.: Composite Structures
 Noryani M., Sapuan S.M., Mastura M.T. et al.: “Stepwise regression for kenaf reinforced polypro pylene composite” in 5th Mechanical Engineering
Research Day 2018, Melaka, Malaysia, May 3, 2018, p. 48.
 Peponi L., Biagiotti J., Torre L. et al.: Polymer Composites
2008, 29, 313.
 Chung K.F., Chiew S.P., Lee H.Y.: “Selection of Equivalent Steel Materials to European Steel Materials Specifications”, Hong Kong Constructional Metal Structures Association, Hong Kong 2015.  Priya I.I.M., Vinayagam B.K.: International Journal of
Polymer Science 2018, ID 8629894.
 Selamat M.Z., Syazwan M., Tahir Z. et al.: “Effect of starch sizes particle as binder on short pineapple leaf fiber composite mechanical properties” in MATEC Web of Conferences 2018, 150, 04008, MUCET 2017 Malaysia.
http://dx.doi.org/10.1051/matecconf/201815004008  Nadlene R., Sapuan S.M., Jawaid M. et al.: BioResources
2016, 11, 9325.
 Sapuan S.M.: “Composite Materials” in “Composite Materials” 1st ed. (Ed. Sapuan S.M.), Butterworth Heinemann: Elsevier Inc., 2017, pp. 57–93.
Received 26 VI 2019.
Serdecznie zapraszamy pracowników uczelni, instytutów badawczych i przemysłu do udziału w
XIV Konferencji Naukowo-Technicznej
„Kierunki Modyfikacji i Zastosowań
połączonej z XXII Warsztatami Profesorskimi,
która odbędzie się w dniach 25–27 maja 2020 r.
w Centrum Postępu Technicznego SIMP w zamku w Rydzynie k. Leszna.
Celem spotkania jest prezentacja i dyskusja naukowa dotycząca przetwórstwa tworzyw polimerowych, ich modyfikacji, metod oceny właściwości oraz nowych zastosowań, a także możliwości współpracy z przemysłem. Wzorem spotkania w 2019 roku (Polimery 2019, 10, 705), planowana jest szeroka dyskusja z udziałem
przedstawicieli przemysłu na temat gospodarki tworzywami polimerowymi w obiegu zamkniętym.
Prof. dr hab. inż. Tomasz Sterzyński
Dr inż. Monika Knitter – email@example.com, tel. 61 6652894
Dr inż. Monika DobrzyńskaMizera – firstname.lastname@example.org, tel. 61 6652894 Biuro Organizacyjne: DIVISIA www.divisia.pl